Seven Ln(III) coordination polymers with two kinds of geometric coordination but the same 3D topological property: luminescence sensing and magnetic property.
Wang, Ai; Zhang, Yatong; Lu, Liping; Zhu, Miaoli; Yuan, Caixia; Feng, Sisi; Dalton transactions (Cambridge, England : 2003) 51 (2022) 12324–12333; doi:10.1039/d2dt01024k

data_7711401
_publ_section_title
;
 Seven Ln(III) coordination polymers with two kinds of geometric
 coordination but the same 3D topological property: luminescence sensing
 and magnetic property.
;
_journal_issue                   32
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              12324
_journal_page_last               12333
_journal_paper_doi               10.1039/d2dt01024k
_journal_volume                  51
_journal_year                    2022
_chemical_formula_moiety         'C18 H13 Eu N9 O8, H2 O'
_chemical_formula_sum            'C18 H15 Eu N9 O9'
_chemical_formula_weight         653.35
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2022-07-19 deposited with the CCDC.	2022-07-21 downloaded from the CCDC.
;
_cell_angle_alpha                83.9876(17)
_cell_angle_beta                 80.5410(18)
_cell_angle_gamma                66.8943(16)
_cell_formula_units_Z            2
_cell_length_a                   9.4618(4)
_cell_length_b                   10.3098(5)
_cell_length_c                   12.4302(6)
_cell_measurement_reflns_used    9254
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.30
_cell_measurement_theta_min      2.66
_cell_volume                     1099.04(9)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT, SADABS and XPREP'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0250
_diffrn_reflns_av_unetI/netI     0.0224
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22567
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.299
_diffrn_reflns_theta_min         2.776
_diffrn_source                   'Incoatec microsource'
_exptl_absorpt_coefficient_mu    2.927
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.6689
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.974
_exptl_crystal_description       block
_exptl_crystal_F_000             642
_exptl_crystal_size_max          0.260
_exptl_crystal_size_mid          0.250
_exptl_crystal_size_min          0.230
_refine_diff_density_max         0.731
_refine_diff_density_min         -1.112
_refine_diff_density_rms         0.090
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.099
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     400
_refine_ls_number_reflns         5431
_refine_ls_number_restraints     195
_refine_ls_restrained_S_all      1.141
_refine_ls_R_factor_all          0.0227
_refine_ls_R_factor_gt           0.0207
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0215P)^2^+1.3001P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0514
_refine_ls_wR_factor_ref         0.0526
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5118
_reflns_number_total             5431
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d2dt01024k2.cif
_cod_data_source_block           EuL66
_cod_database_code               7711401
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.517
_shelx_estimated_absorpt_t_max   0.552
_shelx_res_checksum              56960